surface modiﬁcation of titanium, titanium a lloys,
Post on 21-Jan-2016
Embed Size (px)
Surface modification of titanium, titanium alloys,
and related materials for biomedical applications
Xuanyong Liua,b, Paul K. Chub,*, Chuanxian DingaaShanghai Institute of Ceramics, Chinese Academy of Sciences, 1295 Dingxi Road, Shanghai 200050, ChinabDepartment of Physics and Materials Science, City University of Hong Kong, Tat Chee Avenue,
Kowloon, Hong Kong
Accepted 29 November 2004
Available online 13 January 2005
Titanium and titanium alloys are widely used in biomedical devices and components, especially as hard tissue
replacements as well as in cardiac and cardiovascular applications, because of their desirable properties, such as
relatively low modulus, good fatigue strength, formability, machinability, corrosion resistance, and biocompatibility.
However, titanium and its alloys cannot meet all of the clinical requirements. Therefore, in order to improve the
biological, chemical, and mechanical properties, surface modification is often performed. This article reviews the
various surface modification technologies pertaining to titanium and titanium alloys including mechanical treatment,
thermal spraying, solgel, chemical and electrochemical treatment, and ion implantation from the perspective of
biomedical engineering. Recent work has shown that the wear resistance, corrosion resistance, and biological
properties of titanium and titanium alloys can be improved selectively using the appropriate surface treatment
techniques while the desirable bulk attributes of the materials are retained. The proper surface treatment expands the
use of titanium and titanium alloys in the biomedical fields. Some of the recent applications are also discussed in this
# 2004 Elsevier B.V. All rights reserved.
Keywords: Titanium; Titanium alloys; Surface modification; Biomedical engineering
1.1. Titanium and titanium alloys
Titanium was once considered a rare metal, but nowadays it is one of the most important metals in
the industry. The element was first discovered in England by Gregor in 1790, although it did not
receive its name until Klaproth named it after the mythological first sons of the earth, the Titans, in
1795. Chemically, titanium is one of the transition elements in group IV and period 4 of Mendeleefs
periodic table. It has an atomic number of 22 and an atomic weight of 47.9. Being a transition element,
titanium has an incompletely filled d shell in its electronic structure . Some basic physical properties
of unalloyed titanium are summarized in Table 1. The incomplete shell enables titanium to form solid
solutions with most substitutional elements having a size factor within 20%. In the elemental form,titanium has a high melting point (1668 8C) and possesses a hexagonal closely packed crystal structure
Materials Science and Engineering R 47 (2004) 49121
* Corresponding author. Tel.: +852 27887830; fax: +852 27887724.
E-mail address: email@example.com (X. Liu), firstname.lastname@example.org (P.K. Chu).
0927-796X/$ see front matter # 2004 Elsevier B.V. All rights reserved.doi:10.1016/j.mser.2004.11.001
(hcp) a up to a temperature of 882.5 8C. Titanium transforms into a body centered cubic structure(bcc) b above this temperature .
Titanium alloys may be classified as a, near-a, a + b, metastable b, or stable b depending uponthe room temperature microstructure . In this regard, alloying elements for titanium fall into three
categories: (1) a-stabilizers, such as Al, O, N, C; (2) b-stabilizers, such as Mo, V, Nb, Ta(isomorphous), Fe, W, Cr, Si, Co, Mn, H (eutectoid); (3) neutrals, such as Zr. The a and near-atitanium alloys exhibit superior corrosion resistance but have limited low temperature strength. In
contrast, the a + b alloys exhibit higher strength due to the presence of both the a and b phases. Theproperties of the materials depend on the composition, relative proportions of the a and b phases,thermal treatment, and thermomechanical processing conditions. The b alloys also offer the uniquecharacteristic of low elastic modulus and superior corrosion resistance [4,5].
Titaniumnickel alloy is a stoichiometric compound of Ti and Ni. The equiatomic intermetallic
compound TiNi exhibits the shape memory phenomenon that allows for the spontaneous recovery of
shape after being subjected to macroscopic deformation higher than their elastic limit. Shape recovery
may occur after heating or after release of loads. NiTi shape memory alloy with 55 wt% of Ni and
45 wt% of Ti is often called NITINOL (Ni for nickel, Ti for titanium, and NOL for Naval Ordinance
Laboratory, the place where Buehler and co-workers discovered this alloy). Research activities on the
application of TiNi shape memory alloys to medicine began in the late 1960s to take advantage of
their unique shape memory properties. For example, tailored compressive fixation of bone fragments,
anchoring of implants and dentures to the living tissues, and poisoning of tissues can be more easily
achieved with TiNi alloys. In addition, flexible TiNi stents are increasingly used in surgical treatments
involving constricted arteries, recurrent urethral obstructions, biliary obstructions, and malignant
50 X. Liu et al. / Materials Science and Engineering R 47 (2004) 49121
Summary of physical properties of unalloyed titanium
Atomic number 22
Atomic weight (g/mol) 47.90
Alpha, hexagonal, closely packed
c (A) 4.6832 0.0004a (A) 2.9504 0.0004
Beta, cubic, body centered
a (A) 3.28 0.003Density (g cm3) 4.54Coefficient of thermal expansion, a, at 20 8C (K1) 8.4 106Thermal conductivity (W/(m K)) 19.2
Melting temperature (8C) 1668Boiling temperature (estimated) (8C) 3260Transformation temperature (8C) 882.5
High purity (mV cm) 42Commercial purity (mV cm) 55
Modulus of elasticity, a, (GPa) 105
Yield strength, a, (MPa) 692
Ultimate strength, a, (MPa) 785
1.2. Biomedical applications
Earlier applications of titanium in medical, surgical, and dental devices were based on post-World
War II advances in manufacturing processes as a result of the more stringent requirements demanded
by the aerospace and military industry. Increased use of titanium and its alloys as biomaterials stems
from their lower modulus, superior biocompatibility and better corrosion resistance when compared to
more conventional stainless and cobalt-based alloys. These attractive properties were the driving force
for the early introduction of a (cpTi) and a + b (Ti6Al4V) alloys as well as the more recentdevelopment of modern Ti-based alloys and orthopedic metastable b titanium alloys. The applicationsof titanium and its alloys can be classified according to their biomedical functionalities.
1.2.1. Hard tissue replacements
A schematic diagram of hard tissues in a human body is shown in Fig. 1. Hard tissues are often
damaged due to accidents, aging, and other causes. It is a common practice to surgically substitute the
damaged hard tissues with artificial replacements. Depending on the regions in which the implants are
inserted and the functions to be provided, the requirements of different endoprosthetic materials are
Because of the aforementioned desirable properties, titanium and titanium alloys are widely used
as hard tissue replacements in artificial bones, joints, and dental implants. As a hard tissue
replacement, the low elastic modulus of titanium and its alloys is generally viewed as a biomechanical
advantage because the smaller elastic modulus can result in smaller stress shielding.
One of the most common applications of titanium and its alloys is artificial hip joints that consist
of an articulating bearing (femoral head and cup) and stem as depicted in Fig. 2. The articulating
bearings must be positioned in such a way that they can reproduce the natural movement inside the hip
joints whereas secure positioning of the femoral head in relation to the other components of the joint is
achieved using the stem. The hip stem is anchored permanently to the intramedullary canal of the
femur. The cup, which is the articulating partner of the femoral head, is used for fixation by reaming
out the natural acetabulum to fit the design. Titanium and titanium alloys are also often used in knee
joint replacements, which consist of a femoral component, tibial component, and patella.
X. Liu et al. / Materials Science and Engineering R 47 (2004) 49121 51
Fig. 1. Schematic diagram of hard tissues in human body.
Titanium and titanium alloys are common in dental implants, which can be classified as
subperiosteal, transosteal, and endosseous according to their position and shape. Subperiosteal
implants consist of a custom-cast framework resting on the bone surface beneath the mucoperiosteum.
The prosthesis is secured on posts or abutments that penetrate the mucosa into the oral cavity.
Transosteal implants can only be placed in the frontal lower jaw while endosseous implants can be
placed in both the upper and lower jaws via a mucoperiosteal incision. They are the most commonly
used implant types and can be used in almost any situations as single implants to replace one missing
tooth as well as in cases of partial and total edentulism. The most commonly used endosseous implants
are root-forming analogs. Fig. 3 displays some of the popular designs, suc